Synthesis and Electronic Properties of Conjugated Pentacene Dimers
2008 Vol. 10, No. 21 4779-4782
Dan Lehnherr,† Jianbo Gao,‡ Frank A. Hegmann,*,‡ and Rik R. Tykwinski*,† Department of Chemistry, UniVersity of Alberta, Edmonton, AB T6G 2G2, Canada, and Department of Physics, UniVersity of Alberta, Edmonton, AB T6G 2G7, Canada [email protected]
; [email protected]
Received August 12, 2008
Conjugated pentacene dimers 1-3 were synthesized in two steps from readily available precursors. Noteworthy is the initial step, which assembles five independent fragments to form the carbon-rich molecular framework. Solution-cast films of these materials are air stable. Photocurrent measurements for solution-deposited thin films show that dimer 3 exhibits photoconductive gain >10.
Organic semiconducting materials offer the potential to revolutionize optoelectronics, including applications in photovoltaic cells, chemical sensors, thin film transistors, as well as devices based on nanowires.1 In an effort to provide materials with improved performance for such goals, polyacenes have been a favorite target, building from the wellestablished electronic attributes of anthracene and pentacene.1 One of the biggest breakthroughs in this area has been the development of versatile synthetic protocols to functionalize the pentacene core, and seminal work by Anthony and others have established that such syntheses can provide pentacene derivatives with technologically relevant properties.1,2 An obvious challenge to further improving the overall usefulness of pentacene-based materials would be the forma†
Department of Chemistry. Department of Physics. (1) (a) Bendikov, M.; Wudl, F.; Perepichka, D. F. Chem. ReV. 2004, 104, 4891–4945. (b) Anthony, J. E. Chem. ReV. 2006, 106, 5028–5048. (c) Anthony, J. E. Angew. Chem., Int. Ed. 2008, 47, 452–483. (d) Briseno, A. L.; Mannsfeld, S. C. B.; Jenekhe, S. A.; Bao, Z.; Xia, Y. Mater. Today 2008, 11 (4), 38–47. ‡
10.1021/ol801886h CCC: $40.75 Published on Web 09/30/2008
2008 American Chemical Society
tion of oligomers and polymers that might show enhanced properties. Oligomers also provide an excellent opportunity for assessing structure-property relationships, via comparisons to the corresponding monomeric analogues. Finally, oligomers and polymers also often facilitate the solutionstate deposition of high-quality thin films. Despite these attractive features, pentacene-based oligo- and polymers have, for the most part, remained unrealized until quite recently.3 On the other hand, the study of anthracene oligomers has demonstrated improved conduction versus the corresponding monomers.4 This suggests that the formation of conjugated pentacene oligomers should also afford materi(2) (a) Sheraw, C. D.; Jackson, T. N.; Eaton, D. L.; Anthony, J. E. AdV. Mater. 2003, 15, 2009–2011. (b) Wolak, M. A.; Delcamp, J.; Landis, C. A.; Lane, P. A.; Anthony, J.; Kafafi, Z. AdV. Funct. Mater. 2006, 16, 1943– 1949. (c) Park, J. G.; Vasic, R.; Brooks, J. S.; Anthony, J. E. J. Appl. Phys. 2006, 100, 044511. (d) Park, J. G.; Vasic, R.; Brooks, J. S.; Anthony, J. E. J. Low Temp. Phys. 2006, 142, 391–396. (e) Park, S. K.; Anthony, J. E.; Jackson, T. N. IEEE Electron DeVice Lett. 2007, 28, 877–879. (f) Dickey, K. C.; Subramanian, S.; Anthony, J. E.; Han, L.-H.; Chen, S.; Loo, Y.-L. Appl. Phys. Lett. 2007, 90, 244103. (g) Allard, S.; Forster, M.; Souharce, B.; Thiem, H.; Scherf, U. Angew. Chem., Int. Ed. 2008, 47, 4070–4098.
als with unique and enhanced electronic properties. Herein, we report on the development of a stepwise synthetic route that provides stable, conjugated pentacene dimers 1-3 (Scheme 2). Furthermore, a preliminary study of semicon-
Scheme 2. Synthesis of Pentacene Dimers 1-3
Scheme 1. Synthesis of Model Compound 4
ducting properties of these compounds has been carried out through the analysis of photoconductive gain in comparison to model compounds 4 (Scheme 1) and 5 (Figure 1).
Figure 1. Molecular structure of model compound 5.5
The synthesis of conjugated pentacene dimers necessitated a method of desymmetrization of the core of 6,13-pent(3) (a) Lehnherr, D.; Tykwinski, R. R. Org. Lett. 2007, 9, 4583–4586. (b) Okamoto, T.; Bao, Z. J. Am. Chem. Soc. 2007, 129, 1308–1309. (c) Tokito, S.; Weinfurtner, K.-H.; Fujikawa, H.; Tsutsui, T.; Taga, Y. Proc. SPIE-Int. Soc. Opt. Eng. 2001, 4105, 69–74. (4) (a) Ito, K.; Suzuki, T.; Sakamoto, Y.; Kubota, D.; Inoue, Y.; Sato, F.; Tokito, S. Angew. Chem., Int. Ed. 2003, 42, 1159–1162. (b) Merlo, J. A.; Newman, C. R.; Gerlach, C. P.; Kelley, T. W.; Muyres, D. V.; Fritz, S. E.; Toney, M. F.; Frisbie, C. D. J. Am. Chem. Soc. 2005, 127, 3997– 4009. (c) Kashiwagi, K.; Yasuda, T.; Tsutsui, T. Chem. Lett. 2007, 36, 1194–1195. 4780
acenequinone. A general stepwise approach to unsymmetrical pentacene chromophores has recently been reported and is demonstrated in Scheme 1 for the synthesis of model compound 4.6 In this protocol, the reaction of 6,13pentacenequinone with 1 equiv of lithiated triisopropylsilylacetylene (formed via reaction with HexLi) gave monoaddition product 6 in excellent yield.7,8 The conversion of 6 to diol 7, however, required the use of excess lithiated phenylacetylene due to the presence of the acidic hydroxy group (which quenched 1 equiv of the acetylide). Unfortunately, this procedure is not amenable to the formation of a conjugated dimer. Clearly, the reaction of monoadduct 6 with a diacetylide is problematic given the presence of a hydroxy group, which would only partially quench an incoming diacetylide via protonation. Furthermore, the use of excess (5) For the initial synthesis and study of 5, see: Anthony, J. E.; Brooks, J. S.; Eaton, D. L.; Parkin, S. R. J. Am. Chem. Soc. 2001, 123, 9482–9483. (6) Lehnherr, D.; McDonald, R.; Tykwinski, R. R. Org. Lett. 2008, 10, 4163-4166. (7) Boudebous, A.; Constable, E. C.; Housecroft, C. E.; Neuburger, M.; Schaffner, S. Acta Crystallogr. Sect. C 2006, 62, o243–o245. (8) See Supporting Information for details. Org. Lett., Vol. 10, No. 21, 2008
Figure 2. Spectral data for functionalized pentacenes. (a) Solution-state UV-vis absorption spectra of dimers 1-3 and 4-5 (CH2Cl2). Inset: expansion of low energy absorption region (450-750 nm). (b) Solid-state UV-vis absorption spectra. (c) Photocurrent yield.
diacetylide, as in the transformation of 6 to 7, would not solve this problem. Thus, a one-pot protocol was explored that circumvented the isolation and derivatization of 6. Lithiated triisopropylsilylacetylene was added to a suspension of 6,13-pentacenequinone in THF to form intermediate 6′. This reaction mixture was subsequently added to a solution of lithiated phenylacetylene in THF, and following workup and purification by column chromatography, diol 7 was isolated in excellent yield. Aromatization of 7 using SnCl2·2H2O then gave 4. Compound 4 is highly soluble in, for example, CH2Cl2, CHCl3, and THF, and it can be manipulated under normal laboratory conditions in solution or in the solid state with minimal decomposition. With a viable one-pot procedure in hand, the synthesis of dimers 1-3 followed a similar route. Lithiated trialkylsilylacetylene was added to a suspension of 6,13-pentacenequinone in THF and provided either intermediate 6′ or 8. A solution of this intermediate was then added to the appropriate dilithiated 1,4-diethynylbenzene to complete the dimerization process and afforded pentacene tetraols 9-11 in 17-39% yield. While the isolated yields for 9-11 were moderate to low, it is worth noting that, in a single step, four new carbon-carbon bonds have been formed through the reaction of five individual precursors (equivalent to 64-79% yield per bond forming event). Finally, Sn(II)mediated reduction of 9-11 afforded conjugated pentacene dimers 1-3 in good yields of 72-77%. All dimers could be stored as solids for months under refrigeration in the presence of both air and water without any observable decomposition. Additionally, solutions of these materials could be handled under normal ambient laboratory conditions for several hours with minimal decomposition. The thermal stability of pentacene dimers 1-3 was evaluated by thermal gravimetric analysis (TGA) and differential scanning calorimetry (DSC) in comparison to 4. Although the TGA showed no significant weight loss (10 (i.e., for every photon absorbed, >10 charge carriers traverse the active region of the device).15 This efficiency places spin-cast films of dimer 3 within an order of magnitude of thermally-deposited films of pristine pentacene.16 A plausible explanation for the efficiency of 3, supported by the UV-vis spectroscopic analysis, is that the central Me3Si groups disrupt the planarity of the three aromatic chromophores in the solid state and ultimately reduce the anisotropy of the pentacene chromophores in the film leading to improved efficiency. This is analogous to the improved charge-carrier mobility that is observed in single crystals that have 2-D slipped-stack arrangements vs 1-D stacks.17,18 In conclusion, a new synthetic route to stable, processable pentacene dimers has been developed. The subsequent characterization of photoconductive gain has demonstrated the potential for enhancing electronic properties through synthetic design. The methodology presented provides for future optimization of optoelectronic properties through (a) the use of alternate π-spacers, (b) variation of solubilizing end-groups, and (c) formation of longer pentacene-based oligomers. A full account of these efforts will be reported in due course. Acknowledgment. This work has been generously supported by the University of Alberta and the Natural Sciences and Engineering Research Council of Canada (NSERC) through the Discovery Grant program. We also acknowledge the use of the University of Alberta NanoFab. D.L. thanks NSERC (PGS-D), the Alberta Ingenuity Fund, the University of Alberta, and the Killam Trusts for scholarship support. Supporting Information Available: Experimental procedures, spectroscopic data for new compounds, and AFM images of thin films. This material is available free of charge via the Internet at http://pubs.acs.org. OL801886H (15) For a discussion of the mechanisms of photoconductive gain in organic materials, see ref 13f. (16) Gao, J.; Hegmann, F. A., unpublished results. (17) For acene solid-state packing terminology and its influence on electronic properties, see ref 1b. (18) It is also possible that the variations in film morphology between the different samples also plays a role in efficiency, and this premise is currently being explored.
Org. Lett., Vol. 10, No. 21, 2008